Presentation on theme: "MECHANICAL PROPERTIES OF MATERIALS"— Presentation transcript:
1 MECHANICAL PROPERTIES OF MATERIALS Manufacturing Processes, 1311Dr Simin NasseriSouthern Polytechnic State University
2 MECHANICAL PROPERTIES OF MATERIALS Bending Test (Slide 3)Shear Test (Slide 8)Hardness (Slide 14)Effect of Temperature on Properties (Slide 20)Fluid Properties (Slide 26)Viscoelastic Behavior of Polymers (Slide 34)
4 Bending Test (also called flexure test) Specimen of rectangular cross‑section is positioned between two supports, and a load is applied at its centerFigure Bending of a rectangular cross‑section results in both tensile and compressive stresses in the material: (1) initial loading; (2) highly stressed and strained specimen; and (3) bent part.
6 Testing of Brittle Materials Hard brittle materials (e.g., ceramics) possess elasticity but little or no plasticityOften tested by a bending testBrittle materials do not flexThey deform elastically until fractureFailure occurs because tensile strength of outer fibers of specimen are exceededFailure type: cleavage - common with ceramics and metals at low temperatures, in which separation rather than slip occurs along certain crystallographic planes
7 Transverse Rupture Strength The strength value derived from the bending test:whereTRS = Transverse Rupture Strength;F = applied load at fracture;L = length of specimen between supports; andb and t are dimensions of cross-section
9 Shear Test (also known as torsion test) Application of stresses in opposite directions on either side of a thin elementFigure Shear (a) stress and (b) strain.
10 Shear TestDeform a matchbox and see the deformations in all sides of the box. The area over which the deflection occurs is the area of consideration.AFFA
11 Shear Stress and Strain Shear stress defined aswhere F = applied force; and A = area over which deflection occurs.Shear strain defined aswhere = deflection element; andb = distance over which deflection occurs
12 Torsion Stress-Strain Curve Figure Typical shear stress‑strain curve from a torsion test.
13 Shear Elastic Stress‑Strain Relationship In the elastic region, the relationship is defined aswhere G = shear modulus, or shear modulus of elasticityFor most materials, G 0.4E, where E = elastic modulus
14 Shear Plastic Stress‑Strain Relationship Relationship similar to flow curve for a tensile testShear stress at fracture = shear strength SShear strength can be estimated from tensile strength: S 0.7(TS)Since cross‑sectional area of test specimen in torsion test does not change as in tensile and compression, engineering stress‑strain curve for shear true stress‑strain curve
16 Hardness Resistance to permanent indentation Good hardness generally means material is resistant to scratching and wearMost tooling used in manufacturing must be hard for scratch and wear resistance
17 Hardness TestsCommonly used for assessing material properties because they are quick and convenientVariety of testing methods are appropriate due to differences in hardness among different materialsMost well‑known hardness tests are Brinell and RockwellOther test methods are also available, such as Vickers, Knoop, Scleroscope, and durometer
18 Brinell Hardness TestWidely used for testing metals and nonmetals of low to medium hardnessA hard ball is pressed into specimen surface with a load of 500, 1500, or 3000 kgFigure Hardness testing methods: (a) Brinell
19 Brinell Hardness Number Load divided into indentation area = Brinell Hardness Number (BHN)whereHB = Brinell Hardness Number (BHN),F = indentation load, kg;Db = diameter of ball, mm, andDi = diameter of indentation, mm
20 Brinell Hardness Number Lets work on two extreme cases:Di is extremely low (lets consider it as zero!):This means that if there is almost no indentation, the material is extremely hard!In case Di = Db (the whole ball is inserted into the specimen):A* is the area of the semisphere. This means that HB number is in fact the force divided by the area of contact!
21 Rockwell Hardness Test Figure Hardness testing methods: (b) Rockwell:(1) initial minor load and (2) major load.Another widely used testA cone shaped indenter is pressed into specimen using a minor load of 10 kg, thus seating indenter in materialThen, a major load of 150 kg is applied, causing indenter to penetrate beyond its initial positionAdditional penetration distance d is converted into a Rockwell hardness reading by the testing machine
23 Effect of Temperature on Properties Figure General effect of temperature on strength and ductility.
24 Hot HardnessAbility of a material to retain hardness at elevated temperaturesFigure Hot hardness ‑ typical hardness as a function of temperature for several materials.
25 Recrystallization in Metals Most metals strain-harden at room temperature according to the flow curve (n > 0)But if heated to sufficiently high temperature and deformed, strain hardening does not occurInstead, new grains are formed that are free of strainThe metal behaves as a perfectly plastic material; that is, n = 0
26 Recrystallization Temperature Formation of new strain‑free grains is called recrystallizationRecrystallization temperature of a given metal = about one‑half its melting point (0.5 Tm) as measured on an absolute temperature scaleRecrystallization takes time - the recrystallization temperature is specified as the temperature at which new grains are formed in about one hour
27 Recrystallization and Manufacturing Heating a metal to its recrystallization temperature prior to deformation allows a greater amount of straining, and lower forces and power are required to perform the processForming metals at temperatures above recrystallization temperature is called hot working
29 Fluid Properties and Manufacturing Fluids flow - They take the shape of the container that holds themMany manufacturing processes are accomplished on materials converted from solid to liquid by heatingCalled solidification processesExamples:Metals are cast in molten stateGlass is formed in a heated and fluid statePolymers are almost always shaped as fluids
30 Viscosity in FluidsViscosity is the resistance to flow that is characteristic of a given fluidFlow is a defining characteristic of fluids, but the tendency to flow varies for different fluidsViscosity is a measure of the internal friction when velocity gradients are present in the fluidThe more viscous the fluid, the higher the internal friction and the greater the resistance to flowReciprocal of viscosity is fluidity ‑ the ease with which a fluid flows
31 ViscosityViscosity can be defined using two parallel plates separated by a distance d and a fluid fills the space between the two platesFigure Fluid flow between two parallel plates, one stationary and the other moving at velocity v
32 Shear StressShear stress is the frictional force exerted by the fluid per unit areaMotion of the upper plate is resisted by a frictional force resulting from the shear viscosity of the fluidThis force F can be reduced to a shear stress by dividing by plate area A
33 Shear rate = velocity gradient perpendicular to flow direction Shear stress is related to shear rate, defined as the change in velocity dv relative to dyShear rate = velocity gradient perpendicular to flow directionwhere = shear rate, [1/s];dv = change in velocity, [m/s]; anddy = change in distance y, [m]
34 Shear ViscosityShear viscosity is the fluid property that defines the relationship between F/A and dv/dy; that is,orwhere = a constant of proportionality called the coefficient of viscosity, [Pa-s]For Newtonian fluids, viscosity is a constantFor non-Newtonian fluids, it is not
35 Coefficient of Viscosity Rearranging, Shear viscosity (also called coefficient of viscosity) can be expressed:Viscosity of a fluid is the ratio of shear stress to shear rate during flow
37 Viscosity of Polymers and Flow Rate Viscosity of a thermoplastic polymer melt is not constantIt is affected by flow rateIts behavior is non-NewtonianA fluid that exhibits this decreasing viscosity with increasing shear rate is called pseudoplasticThis complicates analysis of polymer shaping processes such as injection molding
38 Newtonian versus Pseudoplastic Fluids Figure Viscous behaviors of Newtonian and pseudoplastic fluids. Polymer melts exhibit pseudoplastic behavior. For comparison, the behavior of a plastic solid material is shown.
39 Viscoelastic Behavior Material property that determines the strain that the material experiences when subjected to combinations of stress and temperature over timeCombination of viscosity and elasticity
40 Elastic versus Viscoelastic Behavior Figure (a) perfectly elastic response of material to stress applied over time; and (b) response of a viscoelastic material under same conditions. The material in (b) takes a strain that is a function of time and temperature.
41 Viscoelastic Behavior of Polymers: Shape Memory A problem in extrusion of polymers is die swell, in which the profile of extruded material grows in size, reflecting its tendency to return to its previously larger cross section in the extruder barrel immediately before being squeezed through the smaller die opening